Stannous oxide, tin monoxide
|Jmol 3D model||Interactive image|
|Molar mass||134.709 g/mol|
|Appearance||black or red powder when anhydrous, white when hydrated|
|Melting point||1,080 °C (1,980 °F; 1,350 K)|
Std enthalpy of
|Safety data sheet||ICSC 0956|
|US health exposure limits (NIOSH):|
|TWA 2 mg/m3|
IDLH (Immediate danger)
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|what is ?)(|
Tin(II) oxide (stannous oxide) is a compound with the formula SnO. It is composed of tin and oxygen where tin has the oxidation state of +2. There are two forms, a stable blue-black form and a metastable red form.
Preparation and reactions
Blue-black SnO can be produced by heating the tin(II) oxide hydrate, SnO·xH2O (x<1) precipitated when a tin(II) salt is reacted with an alkali hydroxide such as NaOH.
Metastable, red SnO can be prepared by gentle heating of the precipitate produced by the action of aqueous ammonia on a tin(II) salt.
SnO may be prepared as a pure substance in the laboratory, by controlled heating of tin(II) oxalate (stannous oxalate) in the absence of air or under a CO2 atmosphere. This method is also applied to the production of ferrous oxide and manganous oxide.
- Sn(COO)2·2H2O → SnO + CO2 + CO + 2 H2O
- 2 SnO + O2 → 2 SnO2
- 4SnO → Sn3O4 + Sn
- Sn3O4 → 2SnO2 + Sn
SnO is amphoteric, dissolving in strong acid to give tin(II) salts and in strong base to give stannites containing Sn(OH)3−. It can be a dissolves in strong acid solutions to give the ionic complexes Sn(OH2)32+ and Sn(OH)(OH2)2+, and in less acid solutions to give Sn3(OH)42+. Note that anhydrous stannites, e.g. K2Sn2O3, K2SnO2 are also known. SnO is a reducing agent and this appears to its role in the manufacture of so-called "copper ruby glass".
Black, α-SnO adopts the tetragonal PbO layer structure containing four coordinate square pyramidal tin atoms. This form is found in nature as the rare mineral romarchite. The asymmetry is usually simply ascribed to a sterically active lone pair; however, electron density calculations show that the asymmetry is caused by an antibonding interaction of the Sn(5s) and the O(2p) orbitals.
Non-stoichiometry has been observed in SnO.
The dominant use of stannous oxide is as a precursor in manufacturing of other, typically trivalent, tin compounds or salts. Stannous oxide may also be employed as a reducing agent and in the creation of ruby glass- See "Red Glass Coloration - A Colorimetric and Structural Study" By Torun Bring. Pub. Vaxjo University.Red Glass Coloration - A Colorimetric and Structural Study. . It has a minor use as an esterification catalyst.
- Tin and Inorganic Tin Compounds: Concise International Chemical Assessment Document 65, (2005), World Health Organization
- Zumdahl, Steven S. (2009). Chemical Principles 6th Ed. Houghton Mifflin Company. p. A23. ISBN 0-618-94690-X.
- "NIOSH Pocket Guide to Chemical Hazards #0615". National Institute for Occupational Safety and Health (NIOSH).
- Egon Wiberg, Arnold Frederick Holleman (2001) Inorganic Chemistry, Elsevier ISBN 0-12-352651-5
- Satya Prakash (2000),Advanced Inorganic Chemistry: V. 1, S. Chand, ISBN 81-219-0263-0
- Arthur Sutcliffe (1930) Practical Chemistry for Advanced Students (1949 Ed.), John Murray - London.
- The First Oxostannate(II): K2Sn2O3, M Braun, R. Hoppe, Angewandte Chemie International Edition in English, 17, 6, 449 - 450, doi:10.1002/anie.197804491
- Über Oxostannate(II). III. K2Sn2O3, Rb2Sn2O3 und Cs2Sn2O3 - ein Vergleich, R. M. Braun, R. Hoppe, Zeitschrift für anorganische und allgemeine Chemie, 485, 1, 15 - 22, doi:10.1002/zaac.19824850103
- R M Braun R Hoppe Z. Naturforsch. (1982), 37B, 688-694
- Colour development in copper ruby alkali silicate glasses. Part I: The impact of tin oxide, time and temperature ,Bring, T., Jonson, B., Kloo, L. Rosdahl, J , Wallenberg, R., Glass Technology, Eur. J. Glass Science & Technology, Part A, 48 , 2 , 101-108 ( 2007)
- Wells A.F. (1984) Structural Inorganic Chemistry 5th edition Oxford Science Publications ISBN 0-19-855370-6
- On type romarchite and hydroromarchite from Boundary Falls, Ontario, and notes on other occurrences, Robert A. Ramik,, Robert M. Organ, Joseph A. Mandarino, The Canadian Mineralogist; June 2003; v. 41; no. 3;. 649-657; doi:10.2113/gscanmin.41.3.649
- Electronic structures of rocksalt, litharge, and herzenbergite SnO by density functional theory, A. Walsh, G.W. Watson, Phys. Rev. B 70, 235114 (2004)doi:10.1103/PhysRevB.70.235114
- Cation nonstoichiometry in tin-monoxide-phase Sn1-δO with tweed microstructure, Moreno, M. S.; Varela, A.; Otero-Díaz, L. C., Physical Review B (Condensed Matter),56, 9,(1997), 5186-5192, doi:10.1103/PhysRevB.56.5186
- Science and Technology of Chemiresistor Gas Sensors By Dinesh K. Aswal, Shiv K. Gupta (2006), Nova Publishers, ISBN 1-60021-514-9
- "Spectral Studies of New Luminophors for Dental Porcelain" (PDF). Jdr.iadrjournals.org. doi:10.1177/00220345800590090801. Retrieved 2012-04-05.